Journal of Colloid and Interface Science 456 (2015) 206–209
Contents lists available at ScienceDirect
Journal of Colloid and Interface Science journal homepage: www.elsevier.com/locate/jcis
Liposomes as nanoreactors for the photochemical synthesis of gold nanoparticles Sushanth Gudlur 1, Camilla Sandén, Petra Matoušková 2, Chiara Fasciani 3, Daniel Aili ⇑ Division of Molecular Physics, Department of Physics, Chemistry and Biology (IFM), Linköping University, SE-583 36 Linköping, Sweden
g r a p h i c a l a b s t r a c t
Photochemical synthesis of gold nanoparcles in bulk solvent (top panel) and within liposomes (boom panel)
a r t i c l e
i n f o
Article history: Received 13 May 2015 Revised 22 June 2015 Accepted 22 June 2015 Available online 24 June 2015
a b s t r a c t A simple and novel method for the photochemical synthesis of AuNPs in liposomes is described. Gold salt is co-encapsulated with the photoinitiator Irgacure-2959 in POPC liposomes prepared via traditional thin-ﬁlm hydration technique. UVA irradiation for 15 min results in encapsulated AuNPs of 2.8 ± 1.6 nm in diameter that are primarily dispersed in the aqueous interior of the liposomes. Ó 2015 Elsevier Inc. All rights reserved.
Keywords: Liposomes AuNPs Nanoreactors
Gold nanoparticles (AuNPs) have widespread applications in plasmonics , biosensors , electronics , catalysis , ⇑ Corresponding author. E-mail address: [email protected] (D. Aili). Current address: Centre for Biomimetic Sensor Science, School of Materials Science and Engineering, Nanyang Technological University, Singapore 637553, Singapore. 2 Current address: Centre for Materials Research, Faculty of Chemistry, Brno University of Technology, Purkynova 118, 612 00 Brno, Czech Republic. 3 Current address: Istituto Italiano di Tecnologia, Viale Regina Elena 291, 00161 Rome, Italy. 1
http://dx.doi.org/10.1016/j.jcis.2015.06.033 0021-9797/Ó 2015 Elsevier Inc. All rights reserved.
imaging and drug delivery [5,6]. A large number of methods have been developed and optimized for synthesizing AuNPs with deﬁned sizes and shapes [7,8], and typically involves the chemical reduction of Au (III) to Au (0). The initial small clusters of reduced gold thus obtained serve as nucleation sites for the subsequent growth of nanoparticles. For synthesis of spherical AuNPs, besides a reducing agent, an additional stabilizing or capping agent is sometimes added to the reaction mixture to prevent the AuNPs from aggregating. McGilvray et al. , reported a simple and rapid photochemical synthesis of AuNPs to obtain monodisperse spherical nanoparticles that are stable in suspension. In this synthesis,
S. Gudlur et al. / Journal of Colloid and Interface Science 456 (2015) 206–209
the reduction of Au (III) was achieved by ketyl radicals generated due to the UVA-irradiation of Irgacure-2959 (Irg), a photoinitiator. Additionally, the 4-hydroxyethoxy benzoic acid generated from irradiated Irg eventually acts to stabilize the AuNPs and thus prevents them from aggregating. Liposomes are excellent candidates for the compartmentalized synthesis of AuNPs , especially if the end-applications are in the ﬁeld of biological probes and drug delivery. Such compartmentalized synthesis offers the possibility to: control particle size, control the environment of synthesis to include catalytically active components, and carry out synthesis in a highly organized solvent structure . Yet, despite such advantages, previous attempts at synthesizing AuNPs within liposomes have resulted in high size polydispersity, inhomogeneity in shape, or poor yield [12–14]. Recently, the synthesis of AuNPs within liposomes was achieved by the controlled diffusion of stabilizing agents into encapsulated gold salt solutions [15,16], or by doping the lipids that constitute a liposome with glycerol that acts as a reducing agent . However, these approaches have had the need to either modify the method of liposome preparation or use special lipids to achieve controlled synthesis of AuNPs. In this communication, we describe a simple method (Fig. 1) for the controlled synthesis of spherical AuNPs with an average size of 2.8 ± 1.6 nm, inside palmitoyl oleoyl phosphocholine (POPC) liposomes. The resulting AuNPs are homogeneous in size and shape. Moreover, this simple method circumvents the need for separating unencapsulated AuNPs after their synthesis, which can be challenging when employing the more traditional method of encapsulating preformed AuNPs within liposomes. All these, without having to (1) modify existing liposome preparation techniques, (2) introduce additional stabilizing agents in solution, or (3) dope/modify lipids that constitute a liposome, with reducing or stabilizing agents. A freshly prepared solution of HAuCl4 (0.1 mg/mL) and Irg (1 mM) in deionized water was encapsulated into POPC liposomes (2 mg/mL) obtained via the thin-ﬁlm hydration technique  followed by extrusion using a polycarbonate ﬁlter of 100 nm pore size. After removal of unencapsulated HAuCl4 and Irg by separating them over a Sephadex G-25 spin column, the samples were irradiated in a photoreactor with 108 lW/m2 UVA light (365 nm) for 15 min, to generate stable AuNPs within the conﬁnes of the liposome. Photochemical synthesis of AuNPs within liposomes was conﬁrmed by the presence of the localized surface plasmon resonance (LSPR) band centered around 530 nm (Fig. 2). While this LSPR band is typically centered around 520 nm for small (10 nm) and dispersed AuNPs, its position is affected by factors such as particle size, shape, refractive index of the medium, temperature and by species adsorbed on the nanoparticle surface . The position of the LSPR band for AuNPs within liposomes appears red shifted due to the presence of liposomes that scatter signiﬁcantly at lower wavelengths. The effect of liposome scattering on the LSPR peak position was conﬁrmed using liposome encapsulation of commercial AuNPs. In the absence of liposomes they show kmax at 520 nm, and when encapsulated, the peak shifted to kmax 550 nm (Fig. S1). On the other hand, very small AuNPs (
Liposomes as nanoreactors for the photochemical synthesis of gold nanoparticles.
A simple and novel method for the photochemical synthesis of AuNPs in liposomes is described. Gold salt is co-encapsulated with the photoinitiator Irg...